Light Duty: 3.0 kgs/m2
Medium Duty: 5.0 kgs/m2
Heavy Duty: 7 kgs/m2
All surface hardeners are a blend of specialized aggregates and cement binders which may incorporate coloured pigments or be naturally coloured. The pictures above show three typical application rates of a non-metallic traprock aggregate hardener. As you can see, the 3.0kg/m2 [60lb/100sf] "Industry Standard" light application rate has a some spaces between the aggregates, the 5.0kg/m2 [100lb/100sf] medium application rate has less spaces and the 7 kg/m2 [140lb/100sf] heavy application rate has no spaces and the thickness of the hardener has begun to build.
Note that the thickness of a hardener has nothing to do with abrasion resistance. The quality of the aggregate used produces a consistent wear resistance. The thickness of the hardener increases service life only.
The application of surface hardeners is achieved through both hand and mechanical application. Hand application is normally completed after the initial set and floating of the concrete in order to maintain the hardener at the surface of the slab. Mechanical application is commonly performed immediately after concrete placement, before any initial set of the concrete has taken place. Mechanical application is ideal for application rates of 5 kgs/m2 or higher, but are not generally advisable for lower application rates due to concern over the aggregate sinking below the slab surface in the plastic concrete. The maximum application rate by hand is generally 5kgs/m2 (7.5 kgs for mechanical application).
We recommend the following application rates for your consideration:
|End Use:||Application Rate:|
|Foot Traffic||3.0kgs/m2 [60lbs/100sf] OR low water:cement ratio concrete|
|Light Forklift Traffic / Abrasion||3.0 kgs/m2 [60lbs/100sf]|
|Medium Forklift Traffic / Abrasion||5.0 kgs/m2 [100lbs/100sf]|
|Heavy Forklift Traffic / Abrasion||7.0 kgs/m2** [140lbs/100sf]
** Mechanical application is generally required
Material hardness qualities also vary and the following represents the abrasion qualities of various aggregates:
|Metallic Aggregates ##||5||Medium to Heavy Traffic|
|Emery Aggregates||4||Medium to Heavy Traffic|
|Silica Aggregates||3||Light to Medium Traffic|
|Traprock Aggregates||2||Light to Medium Traffic|
|Plain Concrete||1||Light Traffic and Superflat Floors **|
## Metallic aggregates will rust in wet environments.
** Superflat Floors generally do not use surface hardeners due to a reduction in achievable tolerances. Use of a low water:cement ratio concrete mix (maximum 0.50) and a liquid hardener will generally produce suitable abrasion resistance for Superflat environments.
Concrete mixes for interior floors should not include air entrainment and should not have a measured entrapped air content of more than 3% (whether a dry shake hardener is employed or not). Concrete mixes should comply with the recommended mix design considerations (click HERE)
Quality control checks include: (1) the brand and product name of the hardener being applied, (2) the number of bags of material that are on site to install and (3) the number of bags of material actually applied to the surface of the concrete. Most hardener material manufacturers will provide for on-site inspection if requested by the Owner in the specifications.
Full application rates may not be possible in all conditions. Poor access, hot weather conditions and incorrectly designed concrete mixes can make the application of surface hardeners impossible to install at rate of 5kgs/m2 and higher. Surface hardeners are generally used for interior surfaces only.
It is always best to send us an email with your particular circumstances and we will be happy to assist you with your project specification.
70 Leek Crescent, Richmond Hill, Ontario, Canada, L4B 1H1
Tel: (905) 582-9825 Fax: (416) 981-3913